DESIGN OF LAMINATES FOR INPLANE LOADING

 Morris Clark
 3 months ago
 Views:
Transcription
1 DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, Le Mans, France SUMMARY This work relates to the design of laminated structures primarily loaded in membrane, such as pressure vessels. It derives complete formulas, i.e. valid for any loading and any laminate, and without any approximation. Using the so called material ratio and the loading ratio, the design criterion takes a very simple form, equating the two ratios. Keywords: design, laminate, netting theory, polar description of anisotropy, anisotropy. INTRODUCTION Structures primarily loaded in membrane, such as cylindrical pressure vessels, must certainly been considered as the simplest case for design. However even for such cases, the tools available to the designer are on one side the netting theory (NT), which provides explicit design factors but is known to be approximate, and on the other side the classical laminated plate theory (CLPT), which is a precise analysis method, but so requires an iterative process to contribute to a design. As the CLPT in its usual form involves huge algebraic manipulations, it is not possible to derive explicit formulas even for simple cases such as pressurized tubes and only numerical computations can be done. These numerical applications of the CLPT are of course very easy to do and show discrepancy between this CLPT and the netting theory but might not reveal the significant factors for the design. Surprisingly, no work seems to have faced this question of significant parameters until 2002 when Evans and Gibson [1] gave a clear insight into the problem. In order to reveal the factors involved, they succeeded in developing explicit formulas based on the CLPT and compared them to the netting analysis for balanced angleply laminated tubes with hooptoaxialstress ratio of 2:1. They have shown that part of the netting theory can be retained (the principal strains of the plies should be equal), while other parts need to be corrected and they gave a correction formula for the optimal ply angle. Although they had to do lots of tedious algebraic manipulations (Evans [2]), their formulas do not solve exactly the CLPT equations, due to the cumbersome algebra involved in the theory, so their results for the correction in the angle still retain a difference with full calculation. In the numerical examples they published, this correction is shown to be small, however its small value is not guaranteed for other cases and the challenge for an exact CLPT solution remains. To summarize, the limitations of the paper of Evans and Gibson are the following: i) they limited to angleply laminates, ii) they limited to a 2:1 ratio for the principal stresses, iii) their formulas are approximate.
2 METHODOLOGY AND HYPOTHESES For many years, the author has developed the socalled polar method for twodimensional continuum mechanics, using as variables the polar parameters, which are complex linear combinations of the Cartesian components of the stress, strain, stiffness, compliance or other tensors. Among other features, it provides an efficient description of plane anisotropy. So it is useful for twodimensional anisotropic systems such as composite materials. Specially, using these parameters, the CLPT receives an equivalent but simpler form, which makes possible many explicit algebraic developments otherwise intractable. From this, many applications can be derived for analysis and also for design of composites (see for instance [3]). This method was used in the present research, with the aim to improve the results of Evans and Gibson, and suppress their drawbacks. In this part of the paper, we will first describe the loading, geometric and material hypotheses of the study, present some important points of the polar method, then introduce two ratios which are relevant for the present research. In the next part, rules of design will be given, and the design criterion will be derived from them. Structural hypotheses We limit to the simplest conditions for the structure to be designed. Material and geometric hypotheses: the structure is or behaves like a laminated plate. with zero coupling stiffnesses and orthotropic membrane stiffnesses. We will specially consider laminates made of identical plies. Loading hypotheses: the structure is loaded in membrane, with uniform membrane forces N ij. The principal loads are N 1 and N 2, and we limit to the cases with N 1 > N 2 > 0. These hypotheses are those of the netting theory, and notably apply to pressure vessels. Extensions can be made but are not presented here as they make more intricate the discussion, which might conceal the principles of the method, that we want to emphasize. Basics of the polar method Complete equations can be found in [3]. A simpler form is sufficient in the present study. They are presented here in the case of orthotropy and in the principal axes of stress, strain or stiffness: for the stresses or membrane forces, they are obtained from the principal values with major principal axis along direction 1 as: 2 T N 1 N 2 2 R N 1 N 2 and similarly for the strains: 2 t r 1 2
3 for membrane stiffnesses with major principal axis in direction 1, they are: 8 T 0 A A A 1212 A A A 1122 A R 0 A A A 1212 A A 1111 A 2222 Similar formulas hold for ply stiffnesses and for compliances. Loading ratio A loading ratio is defined from the principal membrane forces N 1 > N 2 > 0 as: R T N 1 N 2. N 1 N 2 This quantity will prove to be more relevant to structural design than the more usual ratio N 1/ N 2 (which is the hooptoaxialstress ratio for tubes studied by Evans and Gibson). With the assumed values for the principal loads N k, this material ratio is positive and less than 1. It equals 1/3 in the classical case of cylindrical pressure vessel with hooptoaxialstress ratio equal to 2. Material ratio for the laminate With A ijkl being the inplane stiffnesses, the (inplane) orthotropy axes of the laminate are (1, 2) with the first axis along the direction of the major stiffness: A 1111 > A A material ratio is then defined from two of the polar parameters, as: A 1111 A 2222 A A 1122 A It should be noted that this material ratio does not involve the shear stiffness A Material ratio for a ply A material ratio for any ply is defined similarly from the stiffnesses Q ijkl in the material orthotropy axes (L, T) of the ply : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT This ratio can also be expressed with the compliances S ijkl in the same material orthotropy axes (L, T) or the engineering constants, longitudinal and transverse Young's moduli and, and principal (major) Poisson's ratio ν LT : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT S TTTT S LLLL S LLLL 2 S LLTT S TTTT E 2 LT Notice that this material ratio does not involve the shear property in the orthotropy axes.
4 OVERALL DESIGN PROCESS Design process is split in two steps: first at the laminate level, an overall material satisfying the loading conditions is built, and second, a convenient stacking giving the required overall properties is searched for. Both steps involve the ratios introduced above. Overall design rules We use as overall design criterion the following empirical rules, closely related to the guidelines of the netting analysis: i) select an orthotropic laminate with the major principal axis of stiffness aligned with the major principal axis of the loads, ii) select the material so that the strain is isotropic. Design based on these rules will be consequently called orthotropic isostrain design. Comments of the overall design rules These two rules are neither arbitrary nor obvious. Notice that they do not refer to a definite objective, and are not derived theoretically but are empirical, and so have to be assessed from their consequences. However some rationale is of course behind them. Starting with the meaning of the first rule, it is certainly common sense to retain orthotropic materials with axes aligned with the directions of principal stresses: as the stresses (being a second order tensor) have two orthogonal directions of symmetry, so should have the overall stiffnesses, i.e. the material should be orthotropic (for inplane stiffness properties). Further, the first rule requires that the major orthotropy axis should be along the highest stress and the minor along the lowest stress (remember that the major stiffness is not always along the major stiffness axis, as it may be offaxis, however the stiffness along the major orthotropy axis is always highest than that along the minor orthotropy axis). This point may appear questionable when comparing to the principles of the netting theory, which aims to optimize the structural strength (and in fact cannot meet exactly its assumptions and its aim), while the present formulation appears to rest on elastic behaviour rather to strength behaviour: it is a fact that for an arbitrary orthotropic material, strength and stiffness may differ in orientation and variation. Results for laminates will justify afterwards this rule together with the second rule. As a consequence of the first rule, the strains have the same principal axes than the stresses and stiffnesses, but the major strain may be along any of the principal axes. The second rule settles this point as its meaning is the following: the material should be strained at the same level in any of the principal axes, and consequently in any direction. This second rule is specially relevant for laminates made of identical plies. According to the CLPT, while the state of strain (for membrane loading) is the same through the thickness in the structure axes, it generally varies from ply to ply in the local axes (principal axes of the plies), and so the state of stress in each ply depends on the ply
5 orientation (whatever the axes considered). Only in the case of an isotropic state of strain, the strains are the same in every ply whatever the axes, and consequently the states of stress are the same in the local axes of all the plies: then, every ply is in the same state of strain and stress and so contributes equally to the structural behaviour, which is certainly a good design (and probably an optimal design). Formula of the overall design criterion Translating the design rules in equations is quite simple using the polar parameters. For an orthotropic material loaded in its symmetry axes, the stressstrain relationship, expressed in these symmetry axes with polar parameters, writes: T 4 t 4 r R 4 t 2 T 0 R 0 r Then we have to state that the overall strain is isotropic, that is: r 0 Eliminating t, this gives the design criterion, which expresses simply as the equality of the load and material ratios defined above: R T. The reader can check that this can be derived using the Cartesian components in the orthotropy axes, at the cost of more algebra. STACKING DESIGN PROCESS The previous step of design has defined an overall condition for the material: it must be orthotropic for inplane stiffness, with a fixed value of its material ratio. The next step will be to find stacking sequences meeting these requirements. As an orthotropic laminate possesses 4 independent inplane stiffness parameters, while the material ratio involves only 2 of these parameters, it can be guessed that there might be several solutions. In the following, we examine the common (and simplest) case when the laminate is made of identical plies. Polar method applied to CLPT For laminates made of identical plies, the CLPT equations receive a very simple form with the polar parameters (see [3]). We limit here to the orthotropic case useful for the present research. In this case the 4 polar inplane stiffness parameters have very simple expressions as functions of the polar parameters of the ply. Specially: T t 1 t R 1 cos 2 N k k 1 N
6 where t is the laminate thickness, N is the number of layers and θ k the orientation of the k layer. Consequently, the material ratio of the laminate is equal to the material ratio for the plies /, multiplied by a weighting factor: 1 N N cos2 k k1 It should be noticed that the weighting factor is always less than one. Stacking design equation Substituting in the last equation the value of the loading ratio gives the design equation: R T 1 T N cos 2 1 N k k 1 This equation involves three quantities, the loading ratio of the structure, the material ratio of the ply, and the weighting factor of the stacking sequence. Comments of the stacking design equation The conditions of applicability of our design process appear from this stacking design equation. As the weighting factor is less than 1, solutions can be expected only when: the loading factor should be less than the ply material factor and be at most equal, in which case the only possible solution is a unidirectional material. It can be shown from stability consideration that the material ratio of any material is also less than 1. Table 1 shows typical values for usual unidirectional composites. Table1 : Typical values of the ply material ratio / and polar stiffness parameters for unidirectional reinforcement (T 0,, R 0, in GPa). Material (V f 60%) / T 0 R 0 Eglass /epoxyde HTcarbon /epoxyde HMcarbon /epoxyde The material ratio has two effects. First, when it increases, the range of possible loading is increased too. As said above, the loading ratio range extends to the value of the material ratio, but the effect appears even larger when considering the ratio of the
7 principal stresses instead of the loading ratio. For instance, changing from glass/epoxy plies to HM carbon/epoxy plies increases the material ratio by 40%, and so is the loading ratio range, while the range for the principal stresses ratio is increased by 140%, from 3.8 up to 9. It also can be shown that when the material ratio increases, the formulas get closer to the netting analysis results, and when it goes up to 1, all the formulas reduce to the netting analysis. Using micromechanics formulas of prediction of elastic properties of UD shows that the material ratio is closely dependent on the reinforcementtomatrixstiffness ratio (such as E f /E m ): when this ratio increases, so does the material ratio / of a unidirectionally reinforced ply, up to the limiting case of a very soft matrix (for instance, rubber reinforced with steel fibres), with the ratio going up to 1. Plies reinforced with balanced fabrics have a zero material ratio and cannot be used in our design method. Plies reinforced with unbalanced fabrics have generally a low material ratio, limiting the range of loading they can efficiently carry. When the conditions of applicability are met, several solutions generally exist. The weighting factor should receive a fixed value equal to the loading ratio divided by the ply material ratio, and as it includes an unspecified number N of parameters θ k, an infinite number of solutions exist theoretically. Practical conditions on the number N and the angles values reduce the effective solutions. APPLICATION EXAMPLES To go further, the practical field of design parameters must be specified. Angleply and crossply laminates are of interest. Design of cylindrical pressure vessel is also of major importance for its practical applications as well as for comparison purpose with the netting theory and the Evans and Gibson results. Design with angleply laminates Angleply laminates with layers at ±β (or filament winding in these same directions) are defined by a unique parameter and the design equation writes: cos 2 R T This equation can be solved in seconds with a pocket calculator, to give the optimal angle in agreement with the CLPT. The influence of the significant factors can be check easily. The design angle ±β 0 of the netting theory is given by the limit case when the material ratio equals 1: cos 2 0 R T
8 It appears that cos 2 cos 2 0 so the exact angle is closer to the major stress direction than predicted by the netting theory. A quantitative comparison between these angle values can be obtained by Taylor expansion up to the second order in the quantity (  )/. It gives: 1 1 T /R T 0 1 T /R or using the principal Young's moduli and Poisson's ratio: 1 0 T /R LT 1 1 T / R third order 1 LT third order Design with crossply laminates Crossply laminates are also defined by only one parameter 0 < q < 1, the percentage q of layers at 0, with 1q layers at 90. The design equation writes: 2 q 1 R T So the percentage of plies at 0 should be higher than that indicated by the netting theory, which is such as 2 q 0 1 R /T. Design of cylindrical pressure vessel For cylindrical pressure vessels, N 1 2 N 2, so T 3R. These values in the formulas derived above for angleply laminates define the exact value of the helical angles at which such cylindrical pressure vessels must be wound, angles which are closer to the hoop direction than predicted by the netting theory. The approximate formula derived by Evans and Gibson writes: LT while the present analysis gives: LT LT third order The main difference comes from the term instead of , which appears in the denominator of the Evans and Gibson formula. It explain about 90% of the difference they observed with the numerical results they computed from the CLPT. With the second order terms (in the parentheses) of the present analysis, the CLPT values are recovered exactly.
9 CONCLUSION Within the conditions of applicability of the present approach, all the limitations of the analysis of Evans and Gibson are relieved and explicit design formulas for any state of stress and stacking sequence can be derived. A further step in this research will be to study the stability of solutions obtained. References 1. J T Evans and A G Gibson, 2002, Composite angle ply laminates and netting analysis, Proc. R. Soc. Lond., Vol A 458, pp J T Evans, 2007, private communication ( dated July 6 th, 2007). 3. G Verchery, 1999, Designing with anisotropy, keynote lecture, Twelfth International Conference on Composite Materials (ICCM12), 59 July, Paris.
LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationPEAT SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity
PEAT8002  SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity Nick Rawlinson Research School of Earth Sciences Australian National University Anisotropy Introduction Most of the theoretical
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationANALYSES OF COMPOSITE STRUCTURES. by Stephen W. Tsai, Donald F, Adams, and Douglas R. Doner NASA CR620 REPORT
NASA CONTRACTOR REPORT NASA CR620 sa: 19960410 079 ANALYSES OF COMPOSITE STRUCTURES by Stephen W. Tsai, Donald F, Adams, and Douglas R. Doner & Prepared by PHILCO CORPORATION Newport Beach, Calif. for
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationMathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling
Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationStresses and Strains in flexible Pavements
Stresses and Strains in flexible Pavements Multi Layered Elastic System Assumptions in Multi Layered Elastic Systems The material properties of each layer are homogeneous property at point A i is the same
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. (2015) On tapered warpfree laminates with singleply terminations. Composites Part A: Applied Science and Manufacturing, 72, pp. 127138. Copyright 2015 Elsevier Ltd. A copy can be downloaded
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationCSMA Introduction. M. Brunetti 1, A. Vincenti 2, S. Vidoli 3
CS017 13ème Colloque National en Calcul des Structures 1519 Mai 017, Presqu île de Giens (Var) 13ème Colloque National en Calcul des Structures Multistable shell structures satisfying clamped boundary
More informationChapter 1  Introduction
Chapter 1  Introduction 1.1 Aft pressure bulkhead On a large transport aircraft, the pressurized cabin is closed at the aft end by a domeshaped pressure bulkhead as is shown in Fig. 1.1. In general,
More informationMachine Direction Strength Theory of Corrugated Fiberboard
Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationGerald Allen Cohen, 83, passed away Oct. 1, 2014, at his home in Laguna Beach.
Dr Gerald Allen Cohen (19312014) Ringstiffened shallow conical shell designed with the use of FASOR for NASA s Viking project in the 1970s. (from NASA TN D7853, 1975, by Walter L. Heard, Jr., Melvin
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationA Finite Element Model for Numerical Analysis of Sintering
A Finite Element Model for Numerical Analysis of Sintering DANIELA CÂRSTEA HighSchool Group of Railways, Craiova ION CÂRSTEA Department of Computer Engineering and Communication University of Craiova
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationFormulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading
Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMalaysia Phone: ; Fax:
International Conference on Mechanical Engineering Research (ICMER013), 13 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationBilinear Modelling of Cellulosic Orthotropic Nonlinear Materials
Bilinear Modelling of Cellulosic Orthotropic Nonlinear Materials E.P. SALIKLIS, T.J. URBANIK and B. TOKYAY The proposed method of modelling orthotropic solids that have a nonlinear constitutive material
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More information2 To whom all correspondences should be addressed:
Composite Modeling and Analysis of FDM Prototypes for Design and Fabrication of Functionally Graded Parts Longmei Li, Q. Sun, C. Bellehumeur 1,andP.Gu 2 Department of Mechanical and Manufacturing Engineering
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More information